The influence of hydrothermal fatigue on the clinically relevant functional properties of conventional glass-ionomer cements

During their everyday service, the restorative dental materials are subjected to temperature changes which can be viewed as intensive in the context of the highest allowed temperatures for these materials. In this work, the effect of hydrothermal fatigue on the in vitro tribological performance, compression strength, microhardness, and surface roughness of glass-ionomer cements was studied. Samples of 3 commercially available cements were divided into the reference (aged 14 days) and thermocycled (20,000 cycles; 5–55 °C) groups. The results obtained show that functional properties of the specimens subjected to thermal fatigue significantly differ from the literature data on the cements aged at constant temperatures. The effect of hydrothermal fatigue on the functional properties of cements is discussed in the context of processes induced by exposure to variable temperatures.

www.nature.com/scientificreports/ trials applications, including their time and cost consumption 8 . Moreover, due to large variability in operators, different patient compliance, etc., standardization and replicability of clinical trials are difficult to achieve 8 . Therefore, in vitro testing, which makes it possible to replicate, to some extent, the oral cavity environment and the stresses which are borne both by the teeth and the restorations, is routinely proposed to assess e.g. strength 8 or tribological 9,10 performance of restoratives. However, there is some criticism regarding applicability and robustness of the in vitro tests recommended by the International Organization for Standardization (ISO) [11][12][13] . For example, the ISO tests do not take into account the long-term impact of the oral environment on the maturation processes of GICs. On the other hand, one of the factors which is inevitable during service of a dental restoration is the hydrothermal fatigue 14 . It concerns clinically relevant properties of the restoratives, such as their surface microhardness, compressive strength, or resistance to wear 15 . It is estimated that every day, human oral environment is exposed to action of 20 to 50 thermal cycles 16 . Those are responsible for generating temperature-dependent variable stresses within the polymer matrix of both RBCs and GICs. While polymers are poor conductors of heat, each cycle of heating and subsequent cooling contributes to emergence of thermal stresses at the restorative material's surface. Moreover, the mismatch in coefficient of thermal expansion between the restorative and the tooth contributes to the thermal strain of a restoration 17 . Therefore, to obtain reliable information on the projected long-term behaviour of a restorative dental material in an in vitro test, simulation of hydrothermal fatigue is essential.
To simulate hydrothermal fatigue of dental materials, numerous protocols were developed 8,14,16,18 . One of the first recommendations was included in the 1994's ISO TR 11405 standard 18 , where thermocycling regimen consisting of 500 cycles in water between 5 and 55 °C was suggested 8 . On the other hand, in the protocol presented by Gale and Darvell in 1999 16 , 10,000 thermal cycles in a temperature interval of 35-15-35-45 °C were proposed to simulate 1 year of an in vivo service of a restoration. However, up to date, a great variability in testing methods was seen, including dwell time, temperature range, number of temperatures in the cycle, number of cycles, and others 8,16 . For example, in the works published since 1998, the most popular aging testing method is thermocycling in the temperature range from 5 to 55 °C 8 . However, it has to be noted that, in contrast to resin-based restorative 8,19 and bonding 8,20 materials, the literature on the effect of hydrothermal aging on the properties and performance of glass-ionomers is still scarce [21][22][23][24] . This might be due to the fact that for many years, glass-ionomers were considered suitable mostly for temporary restorations or the non-stress bearing sites 25 . Nevertheless, there are some indications where GICs are used as permanent filling materials, e.g. in atraumatic restorative treatment (ART) 26,27 which is often performed in children 27,28 , and people with disabilities 28 . GICs use in the case of children is highly recommended, because compared to adults, in juvenile patients the occlusal forces are relatively small 27 .
Taking into account the current state of knowledge and the achievements in the clinical applications of glass ionomer cements, the authors of this work conducted an in vitro study on the effect of hydrothermal fatigue on selected functional properties of conventional glass-ionomer cements. The clinically relevant properties, such as: microhardness, compressive strength, tribological performance, and surface roughness, were discussed. The experimental material is enriched with statistical analysis of data, as well as microscopic analyses.

Materials.
Three commercially available self-curing, hand-mixed glass-ionomer cements were used in the study: Ketac Universal, Ketac Molar Easymix (both produced by 3M ESPE, ST. Paul, USA), and Riva Self Cure (SDI Ltd., Bayswater, Australia). For all tested materials, A3 shade was used. All packages of a given type of material had the same LOT number.
According to the manufacturer's data 29 , Ketac Universal (KU) is impermeable to X-rays. It is used to fill cavities in primary and permanent teeth, including, among others, stress bearing sites, cervical areas, Class V, and multi-surface restorations. Moreover, it can be used for tooth core build-up prior to crown placement, fissure sealing, and as a lining for single-and multi-surface composite fillings.
The second tested material was Ketac Molar Easymix (KME) 30 . Its indications for use include semi-permanent Class III and V restorations of primary and permanent teeth, and single-and multi-surface restorations. Additionally, it can be used for restorations of primary teeth, as a liner under composite and amalgam restorations, as well as for cervical fillings without cosmetic priorities. It is impermeable to X-rays.
The third tested material was Riva Self Cure (RSC) 31 . This glass-ionomer cement is used to fill Class I, II and V cavities in permanent teeth, as well as for deciduous teeth restorations. Moreover, it can successfully be used for core build-up, dentine replacement, as well as in temporary fillings, and minimally invasive dentistry. Like the previous two, it is characterized by X-ray permeability. The chemical compositions of all tested materials are shown in Table S1 (Supplementary Information).
It should be emphasized that manufacturers are not obliged to include in their Safety Data Sheets the substances which are deemed harmless. For this reason, the chemical composition of liquid and powder ingredients presented in Supplementary Table S1 shall not be considered fully reliable. For example, in case of KME cement, the manufacturer does not clearly specify the full chemical composition of the liquid 32 . Nevertheless, some evident differences in compositions can be seen, e.g. in tartaric acid content. Usually, 5 to 10 wt% of this acid is used in the liquid ingredient. The tartaric acid is intended to extend the working time and improve setting stage of the material 33 . In addition, powder ingredient of one of the tested cements (KU) does not contain polyacrylic acid.
Sample preparation. The glass-ionomer samples were prepared according to ISO 9917-1 34 and manufacturers' recommendations. GICs were agglutinated in room temperature, by one professional dental operator. Samples were obtained by hand agglutination with a metal spatula on a mixing pad, using the powder and liquid ingredients in ratios recommended by the manufacturers, that is, one level spoonful of powder to one www.nature.com/scientificreports/ drop of aqueous polyacid solution. The cement was placed in the mould immediately after agglutination. After a setting time of 1 h, each sample was transferred to a laboratory incubator set at 37 °C. As a storage medium, deionized water was used. For the measurements of microhardness, surface roughness, friction, and volumetric wear, disc-shaped samples with a diameter of 10 mm and a thickness of 2 mm were made. On the other hand, cylindrical specimens with diameter of 4 mm and a height of 6 mm were used for compressive strength test, as recommended in ISO 9917-1 34 . In total, 6 series of samples were manufactured, and divided into 2 groups. The first one contains reference samples, i.e. not subjected to thermal loads (abbreviations: RSC-Riva Self Cure, KU-Ketac Universal, KME-Ketac Molar Easymix). Those were aged for 14 days in distilled water under constant temperature (37 °C). The latter are the samples subjected to artificial hydrothermal fatigue regimen (abbreviations with suffix TC, e.g. RSC_TC). A summary of the fabricated samples and the number of measurements performed is provided in Supplementary Fig. S1 (online).
Methods. Hydrothermal fatigue. Accelerated hydrothermal fatigue protocol was applied using a laboratory simulator described in 14,35 . The device consisted of a hydraulic module and a microprocessor-based control system. During aging, each sample was placed in a test vessel which was alternately filled with deionized water at 55 °C or 5 °C. One thermal cycle consisted of the following stages: (a) filling the measuring vessel with heated/ cooled water for 10 s; (b) sample dwelling in the heated/cooled water for 30 s; and (c) draining the measuring vessel from the heated/cooled water for 10 s. The dwell time was selected according to related prior publications 8 . For each sample of series 4-6 ( Supplementary Fig. S1), 20,000 hydrothermal cycles were done. In the previous works, it was stated that approximately 10,000 thermal cycles correspond to 1 year of in vivo placement of a dental restoration 8,16 .
Microhardness. Microhardness measurements were carried out according to the Vickers method using a microhardness tester MicVision VH-1 (Sinowon; Dong Guan, China) and a measurement procedure similar to 36 . A load of 200 g was applied, which was equal to a normal force of 1.96 N. For each sample series, n = 16 measurements were taken. The hardness was calculated using the formula: Surface roughness. Using confocal laser microscope, n = 16 line surface roughness measurements were carried out for each series of samples. The sampling length (λ c ) equalled 800 µm, which was the width of the optical field of view obtained with a 20 × lens. It was then taken 5 times for averaging, so that a single evaluation length equalled 4 mm. On the other hand, λ s was set at 2.5 µm in order to exceed the optical resolution of the used lens, and to be equal at least three times of the value of data sampling interval. The following roughness parameters were recorded: the arithmetic average surface roughness Ra, and the mean peak to valley height Rz.
Tribological performance. Wear resistance tests were conducted on a biotribometer (UMT-2, Bruker; Billerica, USA). The experimental conditions were selected as for mastication and oral environment lubrication. A commercial mucin-rich artificial saliva solution was used as a lubricant (Kserostemin, Aflofarm; Poland). The discshaped test sample with a diameter of 10 mm and a height of 2 mm was moving in a reciprocating motion. Teeth shift by of 0.5 mm was assumed, which is close to as reported in 37,38 . Therefore, the length of a friction track was fixed at 500 µm (Fig. S2, Supplementary Information). With regards to the normal load, load of 5 N was chosen, which is in the range of values reported elsewhere 36 for the non-conformal ball-on-disc contacts. As a counter sample, an alumina ball was chosen 39-42 of 6 mm diameter, following 38 . Lastly, a single chewing cycle is estimated to last between 0.87 and 0.95 s 43 , what corresponds to 1 Hz reciprocating frequency and is in line with other in vitro experiments on restoratives 10 . A single measurement lasted 7200 s, while the frequency of sample sliding was set at 1 Hz. Fluctuations in frictional forces over time were acquired a frequency of 10 Hz. For each sample tested, the value of the average coefficient of friction (COF) was calculated, as well as volumetric wear of material was measured. A total of 30 measurements were done, that is, 5 replications for each sample series tested.
(1) www.nature.com/scientificreports/ Microscopic observations. Volumetric wear measurements were conducted by the non-contact method using a laser confocal microscope (CLSM, LEXT4000, Olympus; Tokyo, Japan). In addition, samples were analysed with the use of an SEM-FIB system (Scios 2 DualBeam SEM-FIB, Thermo Fisher Scientific; Waltham, USA). During the studies of both reference GIC microstructures, and the morphology of the wear tracks, the backscatter electron (T1) in-lens detector was used.
Statistical analysis. Statistical analysis of research data was done using Statistica 13.3.0 software for Windows 10 (Statistica 13.3.0, Tibco Software; Palo Alto, USA). The assumption of a normal distribution was checked for all variables using the Shapiro-Wilk test. The null hypothesis was sustained for volumetric wear and surface microhardness data. In order to check the homogeneity of the variances within respective groups, Levene's test was performed. For volumetric wear data, the null hypothesis on the homogeneity of variances was sustained. Therefore, a comparative t test was performed (p < 0.05). On the other hand, for microhardness data, the null hypothesis on the homogeneity of variance was rejected. Therefore, F Welch t test was carried out (p < 0.05). For COF, surface roughness, and compressive strength data, the null hypothesis of normal distribution was rejected (Shapiro-Wilk test, p < 0.05). Thus, differences between respective groups were checked using a U Mann-Whitney test (p < 0.05).

Results
Microstructural analysis of the as-received glass-ionomer samples. The structure of glass-ionomer cements (Fig. 1A) is obtained in a setting reaction between the fluoroaluminosilicate glass particles and the polyacids. In effect, a microstructure of a conventional GIC (Fig. 1B)  Surface roughness. Two surface roughness parameters were analysed: Ra, and Rz. For each of the test series, 16 measurements were taken, and the results are shown in boxplots (Fig. 4). Compared to the reference samples, after thermal fatigue, a decrease in the value of the Ra parameter was found for RSC and KU cements, while for KME, an increase in Ra was seen. Analysis of the Rz parameter has also shown similar differences between the tested groups. It was observed that after hydrothermal aging, the Rz parameter decreased for RSC and KU cements. However, an increase was found for KME glass-ionomer.  www.nature.com/scientificreports/ Tribological performance. Findings from the friction coefficient measurements are shown in Fig. S6 ( Supplementary Information). In each analysed sample series, values of COF were determined from n = 5 measurements. No statistically significant differences in COF between the reference and thermocycled samples were seen. For RSC cement, the scatter of measurement data acquired for fatigued samples was smaller than that of the reference. A similar observation could be done for KME. Although the average COF did not change significantly as a result of fatigue ( Supplementary Fig. S6), differences were observed in the volumetric wear of the tested materials (Fig. 5). For RSC cement, the wear of specimens remained at a similar level, irrespective of the conditioning method. The differences between both groups were found to be statistically insignificant. However, the wear of KU material subjected to thermal loads decreased significantly, whereas substantial increases in wear were observed for KME (paired t test, p < 0.05).
The representative two-dimensional CLSM images of the resultant friction tracks are shown in Fig. 6. All reference samples were characterized by a similar shape of the friction tracks-regular and oval (Figs. 6A-C). However, the differences in shape and size of the friction marks of tested materials obtained before and after hydrothermal aging are noteworthy. For KU cement, after thermocycling, the representative wear track became significantly smaller (Fig. 6E)-shorter and narrower. On the other hand, in case of KME, after hydrothermal aging, the wear track became wider (Fig. 6F). For RSC, a shorter and narrower wear track was seen (Fig. 6D). However, after quantifying volumetric wear, only in RSC no differences were seen (Fig. 5).
To collect information on the dominant wear modes and the wear-and fatigue-induced alterations in the GIC microstructures, high resolution SEM observations were done. In Fig. 7, morphologies of the wear tracks obtained for the reference and thermocycled KU samples are shown. In the reference specimen, two dominant wear modes are present. Tribofilm was formed on the sample surface. It did not adhere well to the frictional track (Fig. 7A). Moreover, abrasive three-body wear of the surface (Fig. 7B) was present. However, after hydrothermal aging, the morphology of the wear track changed. While in Fig. 7A,B no free nano-and microsized wear debris could be seen, in Fig. 7C,D, which represent the fatigued sample, the wear track is covered in free nano-and microparticles. Moreover, signs of tensile cracking of the matrix, were present (Fig. 7C). Nevertheless, after thermocycling, a reduction in volumetric wear of the tested GIC was seen (Fig. 5).
A similar tendency as in KU was seen in KME (Fig. 8). In a reference sample, a tribofilm was formed (Fig. 8A). Some of the glass particles were embedded in the tribofilm, while the others remained free (Fig. 8B). On the other hand, in the fatigued sample (Fig. 8C,D), the elemental contrast between the glass particles and the matrix was poor (Fig. 8C). The wear track was densely covered in micro-and nanometric wear products (Fig. 8D). Moreover, in comparison with the reference (Supplementary Fig. S7A), nanoparticles were not present in the glass particles of fatigued cement (Supplementary Fig. S7B).  www.nature.com/scientificreports/ The least differences in the wear track morphology between the reference and the fatigued samples were seen for Riva Self Cure (Supplementary Fig. S8). In both cases, two main mechanisms of damage of the glass particles are seen: (a) compressive cracking ( Supplementary Fig. S8B,C), and (b) tensile cracking ( Supplementary  Fig. S8B,D). Moreover, flattening-polishing mechanism was seen in both cases. However, wear performance of the material was not affected by the hydrothermal fatigue regimen (Fig. 5).

Discussion
In glass-ionomer cements, the ion-leachable glass (base) reacts with the polyalkenoic acid 47 . In the first, rapid (2-6 min) decomposition phase, neutralization between the acidic polyacid solution and the glass particles takes place 26 . As a consequence, ions such as aluminum, fluoride, calcium, or strontium are being released from the glass particle surface 47 . After the release of the ions, the polyacid molecules become ionized and increase       www.nature.com/scientificreports/ their linearity. Thanks to this, the carboxyl groups of the polyacid are more accessible to ions and facilitate their cross-linking in the later stage of gelation 47 , which is followed by cement setting during which the material properties 26,48 , including microhardness and compressive strength, are developed. The finally cured cement will be a composite of cores of unreacted glass particles, encapsulated in silica gel and embedded in a polyacid-salt matrix that binds the components together 26 . As a consequence of the different types of reinforcing particles used in the commercial formulation, the glass particles used within one GIC may differ in their morphology (Fig. 1A). The manufacturers also ensure that their GICs are impervious to X-rays 29-31 . The bright spots visible on the surface of a representative glass particle (Fig. 1B) are the nanoparticles containing radiocontrast agents. During the maturation stage, which extends to months following the initial setting reaction, various processes take place which result in changes of compressive strength 26,49 , hardness [49][50][51] , toughness 26,49 , wear performance 49 , and opacity of the restorative 26 . The resultant functional properties of GICs, including their mechanical performance [52][53][54][55][56] , and surface state 57,58 , depend on the conditioning environment. Its acidity 54,55 , and chemical composition 55,59 affect the kinetics of the maturation stage, as reflected in the resultant performance of a GIC. When compared with artificial saliva, in deionized and/or distilled water, greater fluoride release [59][60][61] , and mechanical properties 54 , are obtained. This effect results from the inhibitive effect of calcium fluoride deposits 60,61 , which tend to form at the surface of a GIC immersed in an artificial saliva solution 60 . However, no differences are seen in functional properties between the GIC samples stored in deionized or potable water 62 . Nevertheless, most of the available data on maturation processes of GICs concern only early stages of the cements evolution 26 e.g. as evidenced by changes in strength 26 .
Strength (compression, diagonal extension, and/or biaxial flexure) of modern and experimental GICs has been extensively investigated in the "as-formed" state, e.g. 24,[63][64][65] . There is much less information on how these properties change with aging 64,65 . In some studies, mechanical fatigue resistance of GICs was discussed [66][67][68] . Nonetheless, little information can be found on the mechanical in vivo behaviour of GICs, as well as their response to in vitro hydrothermal fatigue or the hydrothermal-mechanical cyclic loading.
It has been suggested that modern GICs behave the same way as traditional cements 49 , reaching the highest strength within a month 26,69,70 . This agrees with reports for modern formulations aged in constant temperature and humidity 64,65,70 . High compressive strength should be beneficial in terms of resistance to wear. However, Mahmood et al. 49 reported that the time evolution of the compressive strength of modern GICs depends on a number of processes which may either positive or negative effect on it. Depending on the relative contribution of these processes, overall strength might undergo changes resisting a simple explanation in particular in the case GICs subjected to thermocycling (Fig. 3).
The compression strength of all tested samples, despite their conditioning method, was over 100 MPa (Figs. 3, S3-S5, Supplementary Information). This is significant from the view of clinical applications of GICs, as according to international standards 34 , compressive strength of 100 MPa or above is required. Our results indicate that hydrothermal fatigue reduces strength of KU and increases of KME. In the case of RSC a slight reduction of compressive strength is statistically insignificant (Fig. 3). It should be noted that similar divergence in changes of the strength has been reported in 24 . An increase in compression strength was found for Fuji IX, another conventional glass-ionomer cement, while for KME, a decrease was reported after hydrothermal aging, however, under 5000 thermal cycles, what equals ¼ of our aging time.
It was previously claimed that decrease of strength in time is typical for acrylic-maleic acid copolymer glassionomers 26 . It is attributed to the fact that acrylic-maleic acid copolymer is characterized by a higher cross-link density than polyacrylic acid, what in the long run makes the cements more brittle compared to the early formulations 71 . However, in our study, all tested cements were acrylic-maleic acid copolymer-based. Moreover, the worst outcome was achieved for the cement in which the polyacrylic acid was not used (KU, Supplementary Table S1). On the other hand, it was found that in higher tartaric-acid GICs, an increased crosslinking density is found due to the action of strongly crosslinking ions, i.e. Al 3+49 . This would explain a far higher median compressive strength of the reference RSC and KU samples in comparison with KME. However, in both RSC and KU, after aging, a reduction in both compressive strength (Fig. 2) and surface microhardness (Fig. 3) was found. This finding corresponds with results obtained by Alrahlah 72 , who reported statistically significant reduction in strength and surface hardness of KU subjected to thermocycling. However, the damaging effect of temperature alterations was seen after only 5000 thermal cycles 72 .
Hardness is one of the properties affecting tribological performance of GICs 50 . Time evolution of hardness of GICs was discussed, e.g. in 51,73 . Nevertheless, there is still ongoing controversy with regard to the effect of long-term hardness on GICs. While conventional GICs stored in water tend to increase their hardness 49,51,65,[73][74][75] , for some new compositions, inverse relationships are reported 44,49,50 . Yet, there are factors that make challenging a direct comparison of the obtained values in different reports 36 . For example, in contrast to our study, the vast majority of the available literature data concerns specimens aged at constant temperatures. Indeed, for the reference samples, we obtained similar hardness as presented in the previously published data (e.g. KME: [75][76][77] ; KU: 65,78 , and RSC: 65 ). Thus, one may explain the increase in post-fatigue hardness presented in Fig. 2 as related to ambient temperature aging.
It occurred that for KME, irrespective of the applied aging protocol, an increase in hardness was found (35% with reference to the control samples, Fig. 2). This agrees with the results of Brito et al. 79 , who reported hardness of KME GIC after 24 h, 30 days and 180 days of storage in distilled water. However, the increase measured in our study was not so spectacular. On the other hand, after hydrothermal aging, for RSC and KU, a substantial decrease in microhardness was found (approx. 18% for KU and 5% for RSC-see Fig. 2). A decrease in hardness of KU subjected to thermocycling was found also in 72 . On the other hand, an increase in hardness of both KU and RSC was found after 7 and 180 days of aging 65 .
In the polyacid-salt matrix of the GIC kit, water exists in two forms: free water particles, which can be removed from the matrix by drying, and bound water particles, which are chemically locked in the matrix 80  www.nature.com/scientificreports/ water plays an important role during cement maturation and ion diffusion 4 , properties of GICs are susceptible to both water uptake, as well as dehydration 81,82 . Moisture contamination reduces the mechanical strength of the restoration and its abrasion resistance, while dehydration causes cracks on the surface of the restorations 82 . It is believed that for a long exposure time, GIC softening phenomena caused by water occur in near-to-surface areas only, not affecting the bulk 50 . However, with regard to studies by De Moor et al. 50 , it could be shown that decrease in surface hardness of samples stored in aqueous media may be attributed to a long-term secondary setting reaction. In this reaction, degradation of glass particles is caused by leaching of siliceous species to form silica gel matrix. This corroborates with the recent studies where the proton 83 and aqueous polyacrylic acid 84 mobility within GICs were discussed. According to Berg et al. 84 , during the maturation stage of a GIC, loose water can become bound, becoming a part of the cement structure, or remain unbound. For some GICs, with aging, the porosity of the material changes 83 , and the volume fraction of the bound water 83 . However, it was presented that GICs tend to increase the content of unbound water in time 80 . While we observed a great contrast in mechanical and tribological performance between the three tested GICs (Figs. 2, 3, and 5) subjected to thermocycling, further research on water mobility is needed to explain quantitively changes in their strength. Surface roughness of the glass-ionomer cements is affected by numerous factors, including, but not limited to: matrix characteristics, size and ratio of glass particles, entrapped air bubbles, and others 85,86 . It was previously reported that in an oral environment, bacterial colonization, plaque formation, and its maturation significantly increase when Ra exceeds 0.2 µm 87 . However, in the cited work 87 , ceramic and metallic implant materials were considered. In our study, all tested GICs were characterized by a much greater roughness (Fig. 4), irrespective of the conditioning methods. Nevertheless, the reported values of Ra were still below the tongue limit of roughness distinction, equal to 0.5 µm 88 . In clinical applications, the increased surface roughness of a dental restoration accounts for, among others, plaque accumulation, secondary caries, and loss of aesthetic properties of a material 89 . Rough surfaces promote proliferation in particular of the bacteria responsible for development of caries (Streptococcus mutans and Lactobacillus spp.) and periodontitis (Porphyromonas gingivalis and Actinobacillosis actinomicetemcomitans) 90 . However, this effect can at least partially be compensated by the fluoride release.
For in vitro wear testing of restorative materials, various techniques and experimental setups are used 10,12,91 , including, but not limited to: Academisch Centrum for Tandheelkunde Amsterdam (ACTA) wear machine 10,91 , OHSU machine 12 , the Alabama machine 12 , the Dento-Munch Robo-Simulator 12 , and others. While the in vitro test rigs are characterized by a remarkable testing efficacy and control over experiment parameters, the great variability in the applied methodologies and operational concepts make it challenging to compare findings obtained by the different authors. Due to this, the in vitro testing is limited mostly to exploration of trends in tribological behaviours of dental restoratives.
Although a limited number of reports on in vitro testing of tribological performance of matured glass-ionomer cements are available, irrespective of the applied testing protocol and used wear measurement methods, for GICs aged in water under constant temperatures, substantial reduction in wear with time is reported 27,49,92 . This trend tends to reverse if samples are subjected to thermocycling 93 . However, in this study, we report that reaction to thermocycling depends on cement composition (Fig. 5). Stable tribological performance was observed in RSC, as proven by the frictional response ( Supplementary Fig. S6), wear (Fig. 5), and morphology of the wear track ( Supplementary Fig. S8). The surface softening phenomenon (Fig. 2), as well as post-fatigue reduction in stiffness of this GIC ( Supplementary Fig. S3), did not affect its long-term wear resistance. On the other hand, even though surface hardness (Fig. 2) and compressive strength (Fig. 3) of KU were deteriorated by the hydrothermal aging, the cement wear resistance improved (Fig. 5). Also, out of all tested GICs, in RSC only, the same dominant wear mechanisms were identified for samples prior to and after thermocycling ( Supplementary  Fig. S8). Surprisingly, the worst long-term tribological performance was observed in the case of samples made of KME, which exhibited high hardness (Fig. 2) and compressive strength (Fig. 3). Finally, it should be noted that in comparison with the reference, in the case of thermocycled KU_TC and KME_TC, size of the wear debris produced as a result of friction decreased from micrometric to submicrometric and nanometric scales (Figs. 7 and 8). The effect of such wear products on the oral tissues is yet unknown.
With regard to statistical analysis of the presented data, one has to be aware of the limitations of the study, in particular the sample sizes (n = 5) in compression strength, COF, and wear measurements. In general, the small sample sizes may subject to type II error, that is, failure to reject the false H 0 hypothesis. In particular the nonparametric tests may be underpowered to detect this. Therefore, further studies are advised.
The findings presented here provide new insights on the hydrothermal phenomena influence on the in vitro performance of GICs. However, one should be aware that this is a relatively new field of investigations and available data on the GICs subjected to thermocycling, in particular their frictional and wear behaviour, are scarce. To our knowledge, this is a first work in which the influence of hydrothermal fatigue on the both clinically relevant mechanical and tribological properties are reported.

Conclusions
Based on the presented findings, the following conclusions are put forward: 1. In contrast to literature data concerning cements aged at constant temperatures, hardness, compressive strength, and wear resistance do not show a consistent increase with time when exposed to temperature cycles. 2. In the case of samples subjected to hydrothermal fatigue, a substantial decrease in the size of wear products, from micrometric to submicrometric and nanometric scales, was found. www.nature.com/scientificreports/ The effect of glass-ionomer cement wear micro-and nano-debris on human oral cavity tissues should be further studied.

Data availability
The datasets generated during and/or analyzed during the current study are available from the corresponding author on reasonable request.